LMucko/crystallography-open-database huggingface dataset:
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517907
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63463(11)
_cell_length_b                   7.63463(11)
_cell_length_c                   7.63463(11)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    20
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.004(11)
_diffrn_ambient_temperature      20
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1093(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.92
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       9.92
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.64
_refine_ls_R_I_factor            1.39
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_20K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.00(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517907
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517908
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63471(12)
_cell_length_b                   7.63471(12)
_cell_length_c                   7.63471(12)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    120
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.018(12)
_diffrn_ambient_temperature      120
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1093(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.86
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       9.94
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.66
_refine_ls_R_I_factor            1.29
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_120K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.02(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517908
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517909
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63536(13)
_cell_length_b                   7.63536(13)
_cell_length_c                   7.63536(13)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    180
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.132(13)
_diffrn_ambient_temperature      180
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1082(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.95
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       10.06
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.75
_refine_ls_R_I_factor            1.24
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_180K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.13(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517909
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517910
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63664(11)
_cell_length_b                   7.63664(11)
_cell_length_c                   7.63664(11)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    300
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.356(11)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1062(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.86
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       9.97
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.68
_refine_ls_R_I_factor            1.23
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_240K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.35(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517910
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517911
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63510(13)
_cell_length_b                   7.63510(13)
_cell_length_c                   7.63510(13)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    160
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.086(13)
_diffrn_ambient_temperature      160
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1087(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.92
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       10.02
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.72
_refine_ls_R_I_factor            1.28
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_160K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.09(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517911
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517912
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63496(13)
_cell_length_b                   7.63496(13)
_cell_length_c                   7.63496(13)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    140
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.062(13)
_diffrn_ambient_temperature      140
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1089(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.84
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       9.98
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.69
_refine_ls_R_I_factor            1.26
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_140K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.06(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517912
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517913
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O12 S Zn4
;
_chemical_formula_sum            'B6 O12 S Zn4'
_chemical_formula_weight         550.48
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.63603(11)
_cell_length_b                   7.63603(11)
_cell_length_c                   7.63603(11)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    220
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     445.249(11)
_diffrn_ambient_temperature      220
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    15.292
_exptl_crystal_density_diffrn    4.1072(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        5.88
_pd_proc_ls_prof_wR_expected     1.30
_pd_proc_ls_prof_wR_factor       9.97
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   7.68
_refine_ls_R_I_factor            1.26
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBOS_220K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        445.249(19)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O12 S Zn4
;
_cod_database_code               4517913